# LAMINATED COMPOSITE PLATES

Size: px
Start display at page:

## Transcription

1 LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA February 10, 2000 Introduction This document is intended to outline the mechanics of fiber-reinforced laminated plates, leading to a computational scheme that relates the in-plane strain and curvature of a laminate to the tractions and bending moments imposed on it. Although this is a small part of the overall field of fiber-reinforced composites, or even of laminate theory, it is an important technique that should be understood by all composites engineers. In the sections to follow, we will review the constitutive relations for isotropic materials in matrix form, then show that the extension to transversely isotropic composite laminae is very straightforward. Since each ply in a laminate may be oriented arbitrarily, we will then show how the elastic properties of the individual laminae can be transformed to a common direction. Finally, we will balance the individual ply stresses against the applied tractions and moments to develop matrix governing relations for the laminate as a whole. The calculations for laminate mechanics are best done by computer, and algorithms are outlined for elastic laminates, laminates exhibiting thermal expansion effects, and laminates exhibiting viscoelastic response. Isotropic linear elastic materials As shown in elementary texts on Mechanics of Materials (cf. Roylance ), the Cartesian strains resulting from a state of plane stress (σ = τ = τ =0)are 1 ɛ = (σ νσ ) 1 ɛ = (σ νσ ) 1 γ = τ In plane stress there is also a strain in the direction due to the Poisson effect: ɛ = ν (σ + σ ); this strain component will be ignored in the sections to follow. In the above relations there are three elastic constants: the Young's modulus, Poisson's ratio ν, and the shear modulus 1 See References listed at the end of this document. 1

2 . However, for isotropic materials there are only two independent elastic constants, and for instance can be obtained from and ν as = 2(1 + ν) Using matrix notation, these relations can be written as > < ɛ => 1 ν/ 0 σ ɛ = 6 > 7 < => ν/ 1 0 σ (1) :> > 4 5 γ ; >: τ >; The quantity in brackets is called the compliance matrix of the material, denoted S or. It is important to grasp the physical significance of its various terms. Directly from the rules of matrix multiplication, the element in the th row and th column of is the contribution of the th stress to the th strain. For instance the component in the 1,2 position is the contribution of the -direction stress to the -direction strain: multiplying σ by 1 gives the -direction strain generated by σ, and then multiplying this by ν gives the Poisson strain induced in the direction. The zero elements show the lack of coupling between the normal and shearing components. If we wish to write the stresses in terms of the strains, Eqn. 1 can be inverted to give: > < σ > = 1 ν 0 ɛ >< > = 6 σ = ν 1 0 ɛ (2) > : > 1 ν τ ; 0 0 (1 ν)2 >: γ >; where here has been replaced by 2(1 + ν). This relation can be abbreviated further as: σ = Dɛ (3) where D = S 1 is the stiffness matrix. Note that the Young's modulus can be recovered by taking the reciprocal of the 1,1 element of the compliance matrix S, but that the 1,1 position of the stiffness matrix D contains Poisson effects and is not equal to. Anisotropic Materials If the material has a texture like wood or unidirectionally-reinforced fiber composites as shown in Fig. 1, the modulus 1 in the fiber direction will typically be larger than those in the transverse directions ( 2 and 3 ). When 1 6= 2 6= 3, the material is said to be orthotropic. It is common, however, for the properties in the plane transverse to the fiber direction to be isotropic to a good approximation ( 2 = 3 ); such a material is called transversely isotropic. The elastic constitutive laws must be modified to account for this anisotropy, and the following form is an extension of the usual equations of isotropic elasticity to transversely isotropic materials: > < ɛ1 = > ν > σ 1 ɛ 2 = 6 7 < >= 4 ν σ2 > : > γ ; :> 12 τ >; 12 The parameter ν 12 is the principal Poisson's ratio; it is the ratio of the strain induced in the 2-direction by a strain applied in the 1-direction. This parameter is not limited to values less than 0.5 as in isotropic materials. Conversely, ν 21 gives the strain induced in the 1-direction by 2 (4)

3 .. Figure 1: An orthotropic material. a strain applied in the 2-direction. Since the 2-direction (transverse to the fibers) usually has much less stiffness than the 1-direction, a given strain in the 1-direction will usually develop a much larger strain in the 2-direction than will the same strain in the 2-direction induce a strain in the 1-direction. Hence we will usually have ν 12 >ν 21. There are five constants in the above equation ( 1, 2, ν 12, ν 21 and 12 ). However, only four of them are independent; since the matrix is symmetric, we have ν 21 2 = ν The simple form of Eqn. 4, with zeroes in the terms representing coupling between normal and shearing components, is obtained only when the axes are aligned along the principal material directions; i.e. along and transverse to the fiber axes. If the axes are oriented along some other direction, all terms of the compliance matrix will be populated, and the symmetry of the material will not be evident. If for instance the fiber direction is off-axis from the loading direction, the material will develop shear strain as the fibers try to orient along the loading direction. There will therefore be a coupling between a normal stress and a shearing strain, which does not occur in an isotropic material. Transformation of Axes It is important to be able to transform the axes to and from the \laboratory" frame to a natural material frame in which the axes might be labeled 1 2 corresponding to the fiber and transverse directions as shown in Fig. 2. Figure 2: Rotation of axes. As shown in elementary textbooks, the transformation law for Cartesian Cauchy stress can 3

4 be written: σ 1 = σ cos 2 θ + σ sin 2 θ +2τ sin θ cos θ σ 2 = σ sin 2 θ + σ cos 2 θ 2τ sin θ cos θ (5) τ12 = 2 2 (σ σ )sinθ cos θ + τ (cos θ sin θ) Where θ is the angle from the axis to the 1 (fiber) axis. These relations can be written in matrix form as <> σ 1 > = 2 > σ 6 σ 2 = < >= σ (6) :> τ ;> >: τ ; > where =cosθand =sinθ. This can be abbreviated as σ 0 = Aσ (7) where A is the transformation matrix in brackets above. This expression could be applied to three-dimensional as well as two-dimensional stress states, although the particular form of A given in Eqn. 6 is valid in two dimensions only (plane stress), and for Cartesian coordinates. Using either mathematical or geometric arguments, it can be shown that the components of infinitesimal strain transform by almost thesamerelations: > < ɛ1 > = >< ɛ >= ɛ 2 = A ɛ (8) >: 1 >; >: 1 γ γ >; The factor of 1/2 on the shear components arises from the classical definition of shear strain, which is twice the tensorial shear strain. This introduces some awkwardness into the transformation relations, which can be reduced by introducing the Reuter's matrix, defined as [R] = or [R] = (9) We can now write: > < ɛ1 => >< ɛ 1 > = >< ɛ >= > < ɛ > = 1 ɛ 2 = R ɛ 2 = RA ɛ = RAR ɛ :> ;> : > 1 > ; > : 1 ; > > γ12 2γ : >; 12 2γ γ Or ɛ 0 = RAR 1 ɛ (10) The transformation law for compliance can now be developed from the transformation laws for strains and stresses. By successive transformations, the strain in an arbitrary - direction is related to strain in the 1-2 (principal material) directions, then to the stresses in the 1-2 directions, and finally to the stresses in the - directions. The final grouping of transformation matrices relating the - strains to the - stresses is then the transformed compliance matrix in the - direction: 2 4

5 > < ɛ >= < > ɛ > = < > ɛ ɛ 1 ɛ = R ɛ = RA 1 1 => <> = > 1 1 ɛ2 = RA R ɛ 2 >: > ; > : 1 >; > : 1 >; >: > γ 2γ 2γ 12 γ ; >< σ 1 => >< σ = RA 1 R 1 = > > < σ => S σ2 = RA 1 R 1 SA σ S σ >: τ >; >: 12 τ >; >: τ ;> where S is the transformed compliance matrix relative to stiffness matrix relative to - axes: - axes. The inverse of S is D, the 1 S = RA 1 R 1 SA D = S (11) Example 1 Consider a ply of Kevlar-epoxy composite with a stiffnesses 1 = 82, 2 =4, 12 =28(allGPa)and ν 12 =025. oriented at 30 from the axis. The stiffness in the direction can be found as the reciprocal of the 1,1 element of the transformed compliance matrix S, as given by Eqn. 11. The following shows how this can be done with Maple symbolic mathematics software (edited for brevity): Read linear algebra package > with(linalg): Define compliance matrix > S:=matrix(3,3,[[1/E[1],-nu[21]/E[2],0],[-nu[12]/E[1],1/E[2],0],[0,0,1/G[12]]]); Numerical parameters for Kevlar-epoxy > Digits:=4;unprotect(E);E[1]:=82e9;E[2]:=4e9;G[12]:=2.8e9;nu[12]:=.25; nu[21]:=nu[12]*e[2]/e[1]; Compliance matrix evaluated > S2:=map(eval,S); := Transformation matrix > A:=matrix(3,3,[[c^2,s^2,2*s*c],[s^2,c^2,-2*s*c],[-s*c,s*c,c^2-s^2]]); Trigonometric relations and angle > s:=sin(theta);c:=cos(theta);theta:=30*pi/180; Transformation matrix evaluated > A2:=evalf(map(eval,A)); := Reuter's matrix > R:=matrix(3,3,[[1,0,0],[0,1,0],[0,0,2]]); Transformed compliance matrix > Sbar:=evalf(evalm( R &* inverse(a2) &* inverse(r) &* S2 &* A2 )); 5

6 := Stiffness in x-direction > 'E[x]'=1/Sbar[1,1]; = Note that the transformed compliance matrix is symmetric (to within numerical roundoff error), but that nonzero coupling values exist. A user not aware of the internal composition of the material would consider it completely anisotropic. Laminated composite plates One of the most common forms of fiber-reinforced composite materials is the crossplied laminate, in which the fabricator \lays up" a sequence of unidirectionally reinforced \plies" as indicated in Fig. 3. Each ply is typically a thin (approximately 0.2 mm) sheet of collimated fibers impregnated with an uncured epoxy or other thermosetting polymer matrix material. The orientation of each ply is arbitrary, and the layup sequence is tailored to achieve the properties desired of the laminate. In this section we outline how such laminates are designed and analyzed. Figure 3: A 3-ply symmetric laminate. \Classical Laminate Theory" is an extension of the theory for bending of homogeneous plates, but with an allowance for in-plane tractions in addition to bending moments, and for the varying stiffness of each ply in the analysis. In general cases, the determination of the tractions and moments at a given location will require a solution of the general equations for equilibrium and displacement compatibility of plates. This theory is treated in a number of standard texts 2,and will not be discussed here. We begin by assuming a knowledge of the tractions N and moments M applied to a plate at a position, as shown in Fig. 4: > < >= < > >= N = M = (12) ;> ;> >: >: 2 cf. S. Timoshenko and S. Woinowsky-Krieger, Theory of Plates and Shells, McGraw-Hill, New York,

7 .. Figure 4: Applied moments in plate bending. It will be convenient to normalize these tractions and moments by the width of the plate, so they have units of N/m and N-m/m, or simply N, respectively. Coordinates and are the directions in the plane of the plate, and is customarily taken as positive downward. The def eflection in the direction is termed, also taken as positive downward... Figure 5: Displacement of a point in a plate (from Powell, 1983). Analogously with the Euler assumption for beams, the Kirshchoff assumption for plate bending takes initially straight vertical lines to remain straight but rotate around the midplane ( = 0). As shown in Fig. 5, the horizontal displacements and in the and directions due to rotation can be taken to a reasonable approximation from the rotation angle and distance from midplane, and this rotational displacement is added to the midplane displacement ( 0 0 ): = 0 0 (13) = 0 0 (14) The strains are just the gradients of the displacements; using matrix notation these can be written 7

8 >< ɛ => >< >= >< 0 0 >= 0 ɛ = ɛ = = 0 0 = ɛ + κ (15) :> >; : > > + ; : > γ (0 + 0 ) 2 >; 0 where ɛ 0 is the midplane strain and κ is the vector of second derivatives of the displacement, called the curvature: > < κ > = >< 0 >= κ = κ = 0 >: κ ; > : > 2 >; 0 The component κ is a twisting curvature, stating how the -direction midplane slope changes with (or equivalently how the -direction slope changes with ). The stresses relative to the - axes are now determined from the strains, and this must take consideration that each ply will in general have a different stiffness, depending on its own properties and also its orientation with respect to the - axes. This is accounted for by computing the transformed stiffness matrix D as described in the previous section (Eqn. 11). Recall that the ply stiffnesses as given by Eqn. 4 are those along the fiber and transverse directions of that particular ply. The properties of each ply must be transformed to a common - axes, chosen arbitrarily for the entire laminate. The stresses at any vertical position are then: σ = Dɛ = Dɛ 0 + Dκ (16) where here D is the transformed stiffness of the ply at the position at which the stresses are being computed. Each of these ply stresses must add to balance the traction per unit width N: Z N = +2 2 Z k σ = X +1 σ (17) =1 k where σ is the stress in the th ply and is the distance from the laminate midplane to the bottom of the th ply. Using Eqn. 16 to write the stresses in terms of the mid-plane strains and curvatures: X (Z k+1 Z k+1 ) N = Dɛ 0 + Dκ (18) =1 k k The curvature κ and midplane strain ɛ 0 are constant throughout, and the transformed stiffness D does not change within a given ply. Removing these quantities from within the integrals: X ( Z k+1 Z ) k+1 N = Dɛ 0 + Dκ =1 k k After evaluating the integrals, this expression can be written in the compact form: where A is an \extensional stiffness matrix" defined as: (19) N = Aɛ 0 + Bκ (20) 8

9 X A = D(+1 ) (21) =1 and B is a \coupling stiffness matrix" defined as: 1 X B = D( ) (22) =1 The rationale for the names \extensional" and \coupling" is suggested by Eqn. 20. The A matrix gives the influ nfluence of an extensional mid-plane strain ɛ 0 on the inplane traction N, and the B matrix gives the contribution of a curvature κ to the traction. It may not be obvious why bending the plate will require an in-plane traction, or conversely why pulling the plate in its plane will cause it to bend. But visualize the plate containing plies all of the same stiffness, except for some very low-modulus plies somewhere above its midplane. When the plate is pulled, the more compliant plies above the midplane will tend to stretch more than the stiffer plies below the midplane. The top half of the laminate stretches more than the bottom half, so it takes on a concave-downward curvature. Similarly, the moment resultants per unit width must be balanced by the moments contributed by the internal stresses: M = Z + 2 σ=bɛ 0 +Dκ (23) 2 where D is a \bending stiffness matrix" defined as: 1 D = X D( ) (24) =1 The complete set of relations between applied forces and moments, and the resulting midplane strains and curvatures, can be summarized as a single matrix equation: ( ) " #( ) N A B ɛ 0 = M B D κ The ABBD matrix in brackets is the laminate stiffness matrix, and its inverse will be the laminate compliance matrix. The presence of nonzero elements in the coupling matrix B indicates that the application of an in-plane traction will lead to a curvature or warping of the plate, or that an applied bending moment will also generate an extensional strain. These effects are usually undesirable. However, they can be avoided by making the laminate symmetric about the midplane, as examination of Eqn. 22 can reveal. (In some cases, this extension-curvature coupling can be used as an interesting design feature. For instance, it is possible to design a composite propeller blade whose angle of attack changes automatically with its rotational speed: increased speed increases the in-plane centripetal loading, which induces a twist into the blade.) The above relations provide a straightforward (although tedious, unless a computer is used) means of determining stresses and displacements in laminated composites subjected to in-plane traction or bending loads: 9 (25)

10 1. For each material type in the stacking sequence, obtain by measurement or micromechanical estimation the four independent anisotropic parameters appearing in Eqn. 4: ( 1, 2, ν 12,and 12 ). 2. Using Eqn. 11, transform the compliance matrix for each ply from the ply's principal material directions to some convenient reference axes that will be used for the laminate as awhole. 3. Invert the transformed compliance matrix to obtain the transformed (relative to - axes) stiffness matrix D. 4. Add each ply's contribution to the A, B and D matrices as prescribed by Eqns. 21, 22 and Input the prescribed tractions N and bending moments M, and form the system equations given by Eqn Solve the resulting system for the unknown values of in-plane strain ɛ 0 and curvature κ. 7. Use Eqn. 16 to determine the ply stresses for each ply in the laminate in terms of ɛ 0, κ and. These will be the stresses relative to the - axes. 8. Use Eqn. 6 to transform the - stresses back to the principal material axes (parallel and transverse to the fibers). 9. If desired, the individual ply stresses can be used in a suitable failure criterion to assess the likelihood of that ply failing. The Tsai-Hill criterion is popularly used for this purpose: ( ) 2 ( ) 2 ( ) σ1 σ 1 σ 2 σ2 τ = 1 (26) σ^1 σ^2 1 σ^2 τ^12 Here σ^1 and σ^2 are the ply tensile strengths parallel to and along the fiber direction, and ^τ 12 is the intralaminar ply strength. This criterion predicts failure whenever the left-hand-side of the above equation equals or exceeds unity. Example 2 The laminate analysis outlined above has been implemented in a code named plate, and this example demonstrates the use of this code in determining the stiffness of a two-ply 0/90 layup of graphite/epoxy composite. Here each of the two plies is given a thickness of 0.5, so the total laminate height will be unity. The laminate theory assumes a unit width, so the overall stiffness and compliance matrices will be based on a unit cross section. > plate assign properties for lamina type 1... enter modulus in fiber direction... (enter -1 to stop): 230e9 enter modulus in transverse direction: 6.6e9 enter principal Poisson ratio:.25 enter shear modulus: 4.8e9 enter ply thickness:.5 assign properties for lamina type

11 enter modulus in fiber direction... (enter -1 to stop): -1 define layup sequence, starting at bottom... (use negative material set number to stop) enter material set number for ply number 1: 1 enter ply angle: 0 enter material set number for ply number 2: 1 enter ply angle: 90 enter material set number for ply number 3: -1 laminate stiffness matrix: E E E D D D E E E D D D E E E D D D E E E D D D E E E D D D E E E D D D+09 laminate compliance matrix: E E E D D D E E E D D D E E E D D D E E E D D D E E E D D D E E E D D D-08 Note that this unsymmetric laminate generates nonzero values in the coupling matrix B, as expected. The stiffness is equal in the and directions, as can be seen by examing the 1,1 and 2,2 elements of the laminate compliance matrix. The effective modulus is = = =392GPa. However, the laminate is not isotropic, as can be found by rerunning plate with the 0/90 layup oriented at a different angle from the axes. Temperature Effects There are a number of improvements one might consider for the plate code described above: it could be extended to include interlaminar shear stresses between plies, it could incorporate a database of commercially available prepreg and core materials, or the user interface could be made \friendlier" and graphically-oriented. Many such features are available in commercial codes, or could be added by the user, and will not be discussed further here. However, thermal expansion effects are so important in application that a laminate code almost must have this feature to be usable, and the general approach will be outlined here. In general, an increase in temperature causes a thermal expansion given by the wellknown relation ɛ = α,whereɛ is the thermally-induced strain and α is the coefficient of 11

12 linear thermal expansion. This thermal strain is obtained without needing to apply stress, so that when Hooke's law is used to compute the stress from the strain the thermal component is subtracted first: σ = (ɛ α ). The thermal expansion causes normal strain only, so shearing components of strain are unaffected. Equation 3 can thus be extended as σ = D (ɛ ɛ ) where the thermal strain vector in the 1 2 coordinate frame is 8 9 > < α 1 >= ɛ = α 2 :> 0 >; Here α 1 and α 2 are the anisotropic thermal expansion coefficients in the fiber and transverse directions. Transforming to common axes, this relation becomes: >< σ => > ɛ σ = 12 α 64 7 < > = ɛ 5 4 α 5 (27) >: > τ ; > : 33 α >; The subscripts on the elements refer to row and column positions within the stiffness matrix rather than coordinate directions; the over-bar serves as a reminder that these elements refer to - axes. The thermal expansion vector on the right-hand side (α = α,α,α ) is essentially a strain vector, and so can be obtained from (α 1,α 2 0) as in Eqn. 10: <> α >= > < α 1 >= α = α = RA 1 R 1 α 2 :> ;> :> 0 >; α Note that in the common - direction, thermal expansion induces both normal and shearing strains. The previous temperature-independent development can now be repeated, modified only by carrying along the thermal expansion terms. As before, the strain vector for any position from the midplane is given in terms of the midplane strain ɛ 0 and curvature κ by The corresponding stress is then σ ɛ = ɛ 0 + κ = D(ɛ 0 + κ α ) Balancing the stresses against the applied tractions and moments as before: Z Z N = σ = Aɛ + Bκ Dα Z M= Z σ=bɛ +Dκ Dα This result is identical to that of Eqns. 20 and 23, other than the addition of the integrals representing the \thermal loads." This permits temperature-dependent problems to be handled by an \equivalent mechanical formulation;" the overall governing equations can be written as 12

13 ( ) " #( ) A B ɛ 0 = N M B D κ or ( ɛ 0 where the \equivalent thermal loads" are given as Z N = N + Dα Z M=M+ κ ) Dα = " A B # 1 ( B D N M ) (28) The extension of the plate code to accommodate thermal effects thus consists of modifying the 6 1 loading vector by adding the two 3 1 vector integrals in the above expression. Viscoelastic Effects Since the matrix of many composite laminates is polymeric, the designer may need to consider the possibility of viscoelastic stress relaxation or creep during loading. Any such effect will probably not be large, since the fibers that bear most of the load are not usually viscoelastic. Further, the matrix material is usually used well below its glass transition temperature, and will act in a glassy elastic mode. Some applications may not be so simple, however. If the laminate is used at elevated temperature, and if stresses act in directions not supported by the reinforcing fibers, relaxation effects may be observed. Figure 6 shows creep measured in a T300/5208 unidirectional graphite-epoxy laminate 3, loaded transversely to the fibers at 149 C. Even in this almost-worst case scenario, the creep strains are relatively small (less than 10% of the elastic strain), but Fig. 6 does show that relaxation effects may be important in some situations. Figure 6: Creep/creep-recovery response of graphite-epoxy laminate. 3 M.E. Tuttle and H.F. Brinson, \Prediction of Long-Term Creep Compliance of General Composite Laminates," Experimental Mechanics, p. 89, March

14 The Tuttle-Brinson paper cited above describes a time-stepping computational scheme that can be used to model these viscoelastic laminate effects, and a simplified form of their method will be outlined here. The viscoelastic creep strain occurring in a given ply during a time increment can be calculated from the stress in the ply at that time, assuming the ply to be free of adjoining plies; this gives an independent-ply creep strain. This strain will act to relax the ply stress. Of course, the plies are not free to strain arbitrarily, and the proper strain compatibility can be reestablished by calculating the external loads that would produce elastic strains equal to the independent-ply creep strains. These loads are summed over all plies in the laminate to give an equivalent laminate creep load. This load is applied to the laminate to compute a set of compatible strains and curvatures, termed the equivalent-laminate creep strain. This strain is added to the initial elastic strain in computing the stress on a given ply, while the independent-ply creep strain is subtracted. The following list develops these steps in more detail: 1. The elastic mid-plane strains and curvatures are solved for the specified bending moments and tractions, using the glassy moduli of the various plies. From Eqn. 25: ( ) " # 1 ɛ 0 A B = κ B D ( N M ) 2. The elastic strain in each ply is then obtained from Eqn. 15. For the ply, with center at coordinate, thisis: 0 ɛ = ɛ + κ where the subscript indicates ply, elastic, strain in the x-y direction. The elastic ply strains relative to the 1-2 (fiber-transverse) directions are given by the transformation of Eqn. 10: ɛ 12 = RAR 1 ɛ These first two steps are performed by the elastic plate code, and the adaptation to viscoelastic response consists of adding the following steps. 3. The current ply stress σ 12 in the 1-2 directions is: σ 12 = D [ɛ 12 +(ɛ 12 ɛ 12 )] The quantity ɛ 12 ɛ 12 is the difference between the equivalent laminate creep strain and the independent-ply creep strain. The quantities ɛ 12 and ɛ 12 are set to zero initially, but are updated in steps 4 and 8 below to account for viscoelastic relaxation. 4. The current ply stress in then used in an appropriate viscoelastic model to compute the creep that would occur if the ply were free to strain independently of the adjoining plies; this is termed the independent ply creep strain. For a simple Voigt model, the current value of creep strain can be updated from its value in the previous time step as: ( ) ɛ = σ 1 dt/τ 1 dt/τ + ɛ where the superscripts on strain indicate values at the current and previous time steps. Here is the viscoelastic creep compliance and τ is a relaxation time. A creep strain 14

15 equal to will develop in addition to the initial elastic strain in the laminate, and a fraction 2 of this creep strain will develop in a time τ. Different values of will be used for the fiber, transverse, and shear strain components due to the anisotropy of the ply. 5. The stresses in the 1-2 and x-y directions that would be needed to develop the independentply creep strains if the ply were elastic are σ σ 12 = Dɛ 12 = A 1 σ These equivalent elastic ply stresses are summed over all plies in the laminate to build up an equivalent laminate creep load. The contribution of the ply is: N = N + σ M = M + σ where is the thickness of the ply and is its centerline coordinate. 7. An equivalent laminate creep strain is then computed from the elastic compliance matrix and the equivalent laminate creep loads as ( ) " # ɛ 0 1 ( ) A B N = κ B D M 8. The ply laminate creep strain in the x-y and 1-2 directions are ɛ ɛ = ɛ 0 + κ 12 = RAR 1 ɛ 9. Finally, the time is incremented ( + ) and another time cycle is computed starting at step 3. Example 3 As an illustration of the above algorithm, consider a simple model laminate with one isotropic ply. The elastic constants are = 100 (arbitrary units) and ν =025, and a unit stress is applied in the -direction. The initial -direction strain is therefore ɛ 0 = σ =001. In this isotropic test case, the code calculates the shear modulus as = 2(1 + ν). The creep strain is governed by a parameter, which sets the Voigt creep compliance to 2 in the transverse direction, 12 for shear components, and zero in the fiber direction (assuming only elastic response along the fibers.) Figure 7 shows the creep strain history of this laminate for a relaxation time of τ = 1000 s. The code steps linearly in log time, in this case with four time steps per decade. The creep strain is the strain over 4 and beyond the initial elastic strain, which transitions from zero to ɛ0 =5 10 as time progresses through the relaxation time. 15

16 Figure 7: Creep strain history in model laminate. References 1. Ashton, J.E., J.C. Halpin and P.H. Petit, Primer on Composite Materials: Analysis,Technomic Press, Westport, CT, Jones, R.M., Mechanics of Composite Materials, McGraw-Hill, New York, Powell, P.C, Engineering with Polymers, Chapman and Hall, London, Roylance, D., Mechanics of Materials, Wiley & Sons, New York, Problems 1. Write out the - two-dimensional compliance matrix S and stiffness matrix D (Eqn. 11) for a single ply of graphite/epoxy composite with its fibers aligned along the - axes. 2. Write out the - two-dimensional compliance matrix S and stiffness matrix D (Eqn. 11) for a single ply of graphite/epoxy composite with its fibers aligned 30 from the axis. 3. Plot the effective Young's modulus, measured along the axis, of a single unidirectional ply of graphite-epoxy composite as a function of the angle between the ply fiber direction and the axis. 4. Using a programming language of your choice, write a laminate code similar to the plate code mentioned in the text, and verify it by computing the laminate stiffness and compliance matrices given in Ex A ( ) layup (the S superscript indicates the plies are repeated to give a symmetric laminate) is an example of what are called \quasi-isotropic" laminates, having equal stiffnesses in the and directions, regardless of the laminate orientation. Verify that this is so for two laminate orientations, one having the 0 plies oriented along the axis and the other with the 0 plies oriented at 30 from the axis. 16

17 Mechanical Properties of Composite Materials The following table lists physical and mechanical property values for representative ply and core materials widely used in fiber-reinforced composite laminates. Ply properties are taken from F.P.Gerstle, \Composites," Encyclopedia of Polymer Science and Engineering, Wiley, New York, 1991, which should be consulted for data from a wider range of materials. See also G. Lubin, Handbook of Composites, Van Nostrand, New York, S-glass/ epoxy Kevlar/ epoxy HM Graphite/ epoxy Pine Rohacell 51 rigid foam Elastic Properties: 1,GPa ,GPa ,GPa ν Tensile Strengths: σ 1,MPa σ 2,Mpa σ 12,MPa Compressive Strengths: σ 1,MPa σ 2,MPa Physical Properties: α 1,10 6 / C α 2,10 6 / C Volume fraction Thickness, mm Density, Mg/m

### LAMINATED COMPOSITE PLATES

LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended

### Constitutive Equations

Constitutive quations David Roylance Department of Materials Science and ngineering Massachusetts Institute of Technology Cambridge, MA 0239 October 4, 2000 Introduction The modules on kinematics (Module

### TABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA

Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1

### Bending of Simply Supported Isotropic and Composite Laminate Plates

Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto Gutierrez-Miravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,

### Module-6: Laminated Composites-II. Learning Unit-1: M6.1. M 6.1 Structural Mechanics of Laminates

Module-6: Laminated Composites-II Learning Unit-1: M6.1 M 6.1 Structural Mechanics of Laminates Classical Lamination Theory: Laminate Stiffness Matrix To this point in the development of classical lamination

### Hygrothermal stresses in laminates

Hygrothermal stresses in laminates Changing environment conditions (temperature and moisture) have an important effect on the properties which are matrix dominated. Change in temperaturet and moisture

### ME 7502 Lecture 2 Effective Properties of Particulate and Unidirectional Composites

ME 75 Lecture Effective Properties of Particulate and Unidirectional Composites Concepts from Elasticit Theor Statistical Homogeneit, Representative Volume Element, Composite Material Effective Stress-

### Composites Design and Analysis. Stress Strain Relationship

Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines

### QUESTION BANK Composite Materials

QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.

### Most of the material in this package is based on a recently published book. This is:

Mechanics of Composite Materials Version 2.1 Bill Clyne, University of Cambridge Boban Tanovic, MATTER Assumed Pre-knowledge It is assumed that the student is familiar with simple concepts of mechanical

### ON THE NUMERICAL ANALYSIS OF COMPOSITE MATERIAL

The 4th International Conference Advanced Composite Materials Engineering COMAT 8- October, Brasov, Romania O THE UMERICAL AALYSIS OF COMPOSITE MATERIAL D.D. icoara Transilvania University, City Brasov,

### Materials and Structures. Indian Institute of Technology Kanpur

Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 34 Thermal Stresses in Plates Lecture Overview Introduction Mechanical and Thermal Strains

### Module 5: Laminate Theory Lecture 17: Laminate Constitutive Relations. The Lecture Contains: Laminate Constitutive Relations

Lecture 17: Laminate Constitutive Relations The Lecture Contains: Laminate Constitutive Relations Classification of Laminates Cross-Ply Laminates Specially Orthotropic Laminates Examples Homework References

### Comparison of Ply-wise Stress-Strain results for graphite/epoxy laminated plate subjected to in-plane normal loads using CLT and ANSYS ACP PrepPost

Comparison of Ply-wise Stress-Strain results for graphite/epoxy laminated plate subjected to in-plane normal loads using CLT and ANSYS ACP PrepPost 1 Mihir A. Mehta, 2 Satyen D. Ramani 1 PG Student, Department

### Module III - Macro-mechanics of Lamina. Lecture 23. Macro-Mechanics of Lamina

Module III - Macro-mechanics of Lamina Lecture 23 Macro-Mechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the

### Passive Damping Characteristics of Carbon Epoxy Composite Plates

Journal of Materials Science and Engineering A 6 (-) 35-4 doi:.765/6-63/6.-.5 D DAVID PUBLISHING Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K * and V V Subba Rao Faculty

### Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA

Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from

DESIGN OF LAMINATES FOR IN-PLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily

### LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS

XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds

### Module 4: Behaviour of a Laminae-II. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites

Module 4: Behaviour of a Laminae-II Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties

### Chapter 2 - Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.

Chapter - Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.

### PROMAL2012 SOFTWARE PACKAGE A USER GUIDE

PROMAL2012 SOFTWARE PACKAGE A USER GUIDE 1. This manual is only for VISTA, WINDOWS 7 and WINDOWS 8 users. The PROMAL2012 software and manual are available at http://www.eng.usf.edu/~kaw/promal2012/ 2.

### Computational Analysis for Composites

Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics

### Effect of Thermal Stresses on the Failure Criteria of Fiber Composites

Effect of Thermal Stresses on the Failure Criteria of Fiber Composites Martin Leong * Institute of Mechanical Engineering Aalborg University, Aalborg, Denmark Bhavani V. Sankar Department of Mechanical

### INTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011

Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.

### FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS

FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Ever J. Barbero Department of Mechanical and Aerospace Engineering West Virginia University USA CRC Press Taylor &.Francis Group Boca Raton London New York

### Exercise: concepts from chapter 8

Reading: Fundamentals of Structural Geology, Ch 8 1) The following exercises explore elementary concepts associated with a linear elastic material that is isotropic and homogeneous with respect to elastic

### Lecture 8. Stress Strain in Multi-dimension

Lecture 8. Stress Strain in Multi-dimension Module. General Field Equations General Field Equations [] Equilibrium Equations in Elastic bodies xx x y z yx zx f x 0, etc [2] Kinematics xx u x x,etc. [3]

### Composite Structural Mechanics using MATLAB

Session 2520 Composite Structural Mechanics using MATLAB Oscar Barton, Jr., Jacob B. Wallace United States Naval Academy Annapolis, Md 21402 Abstract In this paper MATLAB is adopted as the programming

### Module 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains

Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model

### Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)

Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute

### For an imposed stress history consisting of a rapidly applied step-function jump in

Problem 2 (20 points) MASSACHUSETTS INSTITUTE OF TECHNOLOGY DEPARTMENT OF MECHANICAL ENGINEERING CAMBRIDGE, MASSACHUSETTS 0239 2.002 MECHANICS AND MATERIALS II SOLUTION for QUIZ NO. October 5, 2003 For

### CHAPTER 5. Beam Theory

CHPTER 5. Beam Theory SangJoon Shin School of Mechanical and erospace Engineering Seoul National University ctive eroelasticity and Rotorcraft Lab. 5. The Euler-Bernoulli assumptions One of its dimensions

### Stress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina

Chapter 2 Macromechanical Analysis of a Lamina Stress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina Islamic

### A short review of continuum mechanics

A short review of continuum mechanics Professor Anette M. Karlsson, Department of Mechanical ngineering, UD September, 006 This is a short and arbitrary review of continuum mechanics. Most of this material

### VIBRATION AND DAMPING ANALYSIS OF FIBER REINFORCED COMPOSITE MATERIAL CONICAL SHELLS

VIBRATION AND DAMPING ANALYSIS OF FIBER REINFORCED COMPOSITE MATERIAL CONICAL SHELLS Mechanical Engineering Department, Indian Institute of Technology, New Delhi 110 016, India (Received 22 January 1992,

### MECHANICS OF MATERIALS. EQUATIONS AND THEOREMS

1 MECHANICS OF MATERIALS. EQUATIONS AND THEOREMS Version 2011-01-14 Stress tensor Definition of traction vector (1) Cauchy theorem (2) Equilibrium (3) Invariants (4) (5) (6) or, written in terms of principal

### Smart Materials, Adaptive Structures, and Intelligent Mechanical Systems

Smart Materials, Adaptive Structures, and Intelligent Mechanical Systems Bishakh Bhattacharya & Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 19 Analysis of an Orthotropic Ply References

### Course No: (1 st version: for graduate students) Course Name: Continuum Mechanics Offered by: Chyanbin Hwu

Course No: (1 st version: for graduate students) Course Name: Continuum Mechanics Offered by: Chyanbin Hwu 2011. 11. 25 Contents: 1. Introduction 1.1 Basic Concepts of Continuum Mechanics 1.2 The Need

### MITOCW MITRES2_002S10nonlinear_lec15_300k-mp4

MITOCW MITRES2_002S10nonlinear_lec15_300k-mp4 The following content is provided under a Creative Commons license. Your support will help MIT OpenCourseWare continue to offer high quality educational resources

### UNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich

UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST

### VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED - PART 2 )

VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED - PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials

### 6. Bending CHAPTER OBJECTIVES

CHAPTER OBJECTIVES Determine stress in members caused by bending Discuss how to establish shear and moment diagrams for a beam or shaft Determine largest shear and moment in a member, and specify where

### Composite Structures. Indian Institute of Technology Kanpur

Mechanics of Laminated Composite Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 23 Analysis of an Orthotropic Ply Lecture Overview Introduction Engineering constants for an 2

### 2. Mechanics of Materials: Strain. 3. Hookes's Law

Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate

### Cellular solid structures with unbounded thermal expansion. Roderic Lakes. Journal of Materials Science Letters, 15, (1996).

1 Cellular solid structures with unbounded thermal expansion Roderic Lakes Journal of Materials Science Letters, 15, 475-477 (1996). Abstract Material microstructures are presented which can exhibit coefficients

### Open-hole compressive strength prediction of CFRP composite laminates

Open-hole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr

### Composite models 30 and 131: Ply types 0 and 8 calibration

Model calibration Composite Bi-Phase models 30 and 3 for elastic, damage and failure PAM-CRASH material model 30 is for solid and 3 for multi-layered shell elements. Within these models different ply types

### MODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE

MODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE Jean Paul Charles, Christian Hochard,3, Pierre Antoine Aubourg,3 Eurocopter, 375 Marignane cedex, France Unimeca, 6 rue J. Curie, 3453

### Fracture Mechanics, Damage and Fatigue: Composites

University of Liège Aerospace & Mechanical Engineering Fracture Mechanics, Damage and Fatigue: Composites Ludovic Noels Computational & Multiscale Mechanics of Materials CM3 http://www.ltas-cm3.ulg.ac.be/

### STRESSES WITHIN CURVED LAMINATED BEAMS OF DOUGLAS-FIR

UNITED STATES DEPARTMENT OF AGRICULTURE. FOREST SERVICE - FOREST PRODUCTS LABORATORY - MADISON, WIS. STRESSES WITHIN CURVED LAMINATED BEAMS OF DOUGLAS-FIR NOVEMBER 1963 FPL-020 STRESSES WITHIN CURVED LAMINATED

### Passive Damping Characteristics of Carbon Epoxy Composite Plates

Journal of aterials Science and Engineering A 6 (1-2) (2016) 35-42 doi: 10.17265/2161-6213/2016.1-2.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K

### As an example we consider the stacking and analysis of a 2-ply symmetric laminate. First we clear the Matlab space and close figures.

Program Lam 1 Introduction The collection of Matlab command and function files in the package lam allows the stacking and analysis of a laminate. In fact only a representative piece of a laminate is considered,

### PURE BENDING. If a simply supported beam carries two point loads of 10 kn as shown in the following figure, pure bending occurs at segment BC.

BENDING STRESS The effect of a bending moment applied to a cross-section of a beam is to induce a state of stress across that section. These stresses are known as bending stresses and they act normally

### THE NETTING ANALYSIS AS A LIMIT CASE OF THE LAMINATED STRUCTURE THEORY

THE NETTING ANALYSIS AS A LIMIT CASE OF THE LAMINATED STRUCTURE THEORY G. Verchery Pluralis, Saint-Étienne, France Georges.Verchery@m4x.org Keywords: netting analysis, classical laminated plate theory,

### PLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE

7th European Workshop on Structural Health Monitoring July 8-11, 2014. La Cité, Nantes, France More Info at Open Access Database www.ndt.net/?id=17206 PLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE

### Practice Final Examination. Please initial the statement below to show that you have read it

EN175: Advanced Mechanics of Solids Practice Final Examination School of Engineering Brown University NAME: General Instructions No collaboration of any kind is permitted on this examination. You may use

### Dynamic Analysis of Laminated Composite Plate Structure with Square Cut-Out under Hygrothermal Load

Dynamic Analysis of Laminated Composite Plate Structure with Square Cut-Out under Hygrothermal Load Arun Mukherjee 1, Dr. Sreyashi Das (nee Pal) 2 and Dr. A. Guha Niyogi 3 1 PG student, 2 Asst. Professor,

### Elements of Continuum Elasticity. David M. Parks Mechanics and Materials II February 25, 2004

Elements of Continuum Elasticity David M. Parks Mechanics and Materials II 2.002 February 25, 2004 Solid Mechanics in 3 Dimensions: stress/equilibrium, strain/displacement, and intro to linear elastic

### Advanced Structural Analysis EGF Section Properties and Bending

Advanced Structural Analysis EGF316 3. Section Properties and Bending 3.1 Loads in beams When we analyse beams, we need to consider various types of loads acting on them, for example, axial forces, shear

### Laminated Beams of Isotropic or Orthotropic Materials Subjected to Temperature Change

United States Department of Agriculture Forest Service Forest Products Laboratory Research Paper FPL 375 June 1980 Laminated Beams of Isotropic or Orthotropic Materials Subjected to Temperature Change

### MECHANICS OF COMPOSITE STRUCTURES

MECHANICS OF COMPOSITE STRUCTURES LÁSZLÓ P. KOLLÁR Budapest University of Technology and Economics GEORGE S. SPRINGER Stanford University PUBLISHED BY THE PRESS SYNDICATE OF THE UNIVERSITY OF CAMBRIDGE

### Lab Exercise #5: Tension and Bending with Strain Gages

Lab Exercise #5: Tension and Bending with Strain Gages Pre-lab assignment: Yes No Goals: 1. To evaluate tension and bending stress models and Hooke s Law. a. σ = Mc/I and σ = P/A 2. To determine material

### ME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)

ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,

### Presented By: EAS 6939 Aerospace Structural Composites

A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have

### Using MATLAB to Design and Analyse Composite Laminates

Engineering, 2010, 2, 904-916 doi:10.4236/eng.2010.211114 Published Online November 2010 (http://www.scirp.org/journal/eng). Using MATLAB to Design and Analyse Composite Laminates Abstract Avinash Ramsaroop,

### Effect of Specimen Dimensions on Flexural Modulus in a 3-Point Bending Test

Effect of Specimen Dimensions on Flexural Modulus in a 3-Point Bending Test M. Praveen Kumar 1 and V. Balakrishna Murthy 2* 1 Mechanical Engineering Department, P.V.P. Siddhartha Institute of Technology,

### Failure Analysis of Unidirectional Composite Pinned- Joints

217 IJEDR Volume, Issue 4 ISSN: 2321-9939 Failure Analysis of Unidirectional Composite Pinned- Joints 1 Sai Ashok.M, 2 Mr. U. Koteswara Rao 1 M-tech Machine Design, 2 Associate Professor & Asst. COE 1

### five Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture

ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS

### Predicting Failure of Multiangle Composite Laminates

Predicting Failure of Multiangle Composite Laminates Preliminary discussion (not in textbook): Micromechanics failure analyses vs Macromechanics failure analyses Fiber Architecture of Some Common Composite

### Composite Laminate Modeling

omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER

### Classical Lamination Theory: The Kirchhoff Hypothesis

212 Chapter 6 Classical Lamination Theory: The Kirchhoff Hypothesis In the preceding chapters we developed the tools needed to understand the elastic response of a small volume of fiber-reinforced material

### Micromechanical analysis of FRP hybrid composite lamina for in-plane transverse loading

Indian Journal of Engineering & Materials Sciences Vol. 15, October 2008, pp. 382-390 Micromechanical analysis of FRP hybrid composite lamina for in-plane transverse loading K Sivaji Babu a *, K Mohana

### Modelling the nonlinear shear stress-strain response of glass fibrereinforced composites. Part II: Model development and finite element simulations

Modelling the nonlinear shear stress-strain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent

### Module 5: Laminate Theory Lecture 19: Hygro -thermal Laminate Theory. Introduction: The Lecture Contains: Laminate Theory with Thermal Effects

Module 5: Laminate Theory Lecture 19: Hygro -thermal Laminate Theory Introduction: In this lecture we are going to develop the laminate theory with thermal and hygral effects. Then we will develop the

### Chapter 2: Elasticity

OHP 1 Mechanical Properties of Materials Chapter 2: lasticity Prof. Wenjea J. Tseng ( 曾文甲 ) Department of Materials ngineering National Chung Hsing University wenjea@dragon.nchu.edu.tw Reference: W.F.

### MESH MODELING OF ANGLE-PLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP

16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLE-PLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic

### 202 Index. failure, 26 field equation, 122 force, 1

Index acceleration, 12, 161 admissible function, 155 admissible stress, 32 Airy's stress function, 122, 124 d'alembert's principle, 165, 167, 177 amplitude, 171 analogy, 76 anisotropic material, 20 aperiodic

### 3.22 Mechanical Properties of Materials Spring 2008

MIT OpenCourseWare http://ocw.mit.edu 3.22 Mechanical Properties of Materials Spring 2008 For information about citing these materials or our Terms of Use, visit: http://ocw.mit.edu/terms. Quiz #1 Example

### The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints

, June 30 - July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed

### Stacking sequences for Extensionally Isotropic, Fully Isotropic and Quasi-Homogeneous Orthotropic Laminates.

49th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials 7-10 April 2008, Schaumburg, IL AIAA 2008-1940 Stacking sequences for Extensionally Isotropic, Fully Isotropic and Quasi-Homogeneous

### Failure analysis of serial pinned joints in composite materials

Indian Journal of Engineering & Materials Sciences Vol. 18, April 2011, pp. 102-110 Failure analysis of serial pinned joints in composite materials Alaattin Aktaş* Department of Mechanical Engineering,

### VYSOKÁ ŠKOLA BÁŇSKÁ TECHNICKÁ UNIVERZITA OSTRAVA

VYSOKÁ ŠKOLA BÁŇSKÁ TECHNICKÁ UNIVERZITA OSTRAVA FAKULTA METALURGIE A MATERIÁLOVÉHO INŽENÝRSTVÍ APPLIED MECHANICS Study Support Leo Václavek Ostrava 2015 Title:Applied Mechanics Code: Author: doc. Ing.

### Chapter 3. Load and Stress Analysis

Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3

### Structural Dynamics Lecture Eleven: Dynamic Response of MDOF Systems: (Chapter 11) By: H. Ahmadian

Structural Dynamics Lecture Eleven: Dynamic Response of MDOF Systems: (Chapter 11) By: H. Ahmadian ahmadian@iust.ac.ir Dynamic Response of MDOF Systems: Mode-Superposition Method Mode-Superposition Method:

### SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS

SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATEC-SP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS

### Tuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE

1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & Free-Body Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for

### MECHANICS OF MATERIALS

CHATR Stress MCHANICS OF MATRIALS and Strain Axial Loading Stress & Strain: Axial Loading Suitability of a structure or machine may depend on the deformations in the structure as well as the stresses induced

### Mechanics PhD Preliminary Spring 2017

Mechanics PhD Preliminary Spring 2017 1. (10 points) Consider a body Ω that is assembled by gluing together two separate bodies along a flat interface. The normal vector to the interface is given by n

### Linear elastic analysis of thin laminated beams with uniform and symmetric cross-section

Applied and Computational Mechanics 2 (2008) 397 408 Linear elastic analysis of thin laminated beams with uniform and symmetric cross-section M. Zajíček a, a Faculty of Applied Sciences, UWB in Pilsen,

### Basic Energy Principles in Stiffness Analysis

Basic Energy Principles in Stiffness Analysis Stress-Strain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting

### Fracture Mechanics of Composites with Residual Thermal Stresses

J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate

### Learning Units of Module 3

Module Learning Units of Module M. tress-train oncepts in Three- Dimension M. Introduction to Anisotropic lasticity M. Tensorial oncept and Indicial Notations M.4 Plane tress oncept Action of force (F)

### Materials and Structures. Indian Institute of Technology Kanpur

Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional

### Elements of Polymer Structure and Viscoelasticity. David M. Parks Mechanics and Materials II February 18, 2004

Elements of Polymer Structure and Viscoelasticity David M. Parks Mechanics and Materials II 2.002 February 18, 2004 Outline Elements of polymer structure Linear vs. branched; Vinyl polymers and substitutions

### Module 7: Micromechanics Lecture 25: Strength of Materials Approach. Introduction. The Lecture Contains. Effective Transverse Modulus

Introduction In the previous lecture we have introduced the concept of Representative Volume Element or Unit Cell. This is the basic building block in a micromechanical study. Further, we explained the

### MATERIAL PROPERTIES. Material Properties Must Be Evaluated By Laboratory or Field Tests 1.1 INTRODUCTION 1.2 ANISOTROPIC MATERIALS

. MARIAL PROPRIS Material Properties Must Be valuated By Laboratory or Field ests. INRODUCION he fundamental equations of structural mechanics can be placed in three categories[]. First, the stress-strain

### Mechanical Engineering Ph.D. Preliminary Qualifying Examination Solid Mechanics February 25, 2002

student personal identification (ID) number on each sheet. Do not write your name on any sheet. #1. A homogeneous, isotropic, linear elastic bar has rectangular cross sectional area A, modulus of elasticity